2Department of Physics and Astronomy and Ames Laboratory, Iowa State University, ... 3Applied Optics Beijing Area Major Laboratory, Department of Physics, ...
Chiral metamaterials with negative refractive index based on four “U” split ring resonators Zhaofeng Li,1 Rongkuo Zhao,2,3 Thomas Koschny,2,4 Maria Kafesaki,4 Kamil Boratay Alici,1 Evrim Colak,1 Humeyra Caglayan,1 Ekmel Ozbay1,5 and C. M. Soukoulis,2,4,a) 1
Nanotechnology Research Center, and Department of Physics, Bilkent University, Bilkent, 06800 Ankara,
Department of Physics and Astronomy and Ames Laboratory, Iowa State University, Ames, Iowa 50011, USA
Applied Optics Beijing Area Major Laboratory, Department of Physics, Beijing Normal University, Beijing
100875, China 4
Institute of Electronic Structure and Laser, Foundation for Research and Technology Hellas (FORTH), and
Department of Materials Science and Technology, University of Crete, 71110 Heraklion, Greece 5
Nanotechnology Research Center, Department of Physics, and Department of Electrical and Electronics
Engineering, Bilkent University, Bilkent, 06800 Ankara, Turkey A uniaxial chiral metamaterial is constructed by double-layered four “U” split ring resonators mutually twisted by 90 degrees. It shows a giant optical activity and circular dichroism. The retrieval results reveal that a negative refractive index is realized for circularly polarized waves due to the large chirality. The experimental results are in good agreement with the numerical results. Chiral metamaterials (CMMs) have attracted much
where ε0 and μ0 are the permittivity and permeability of
attention ever since it was predicted that negative refraction
vacuum. ε and μ are the relative permittivity and permeability of the chiral medium. c is the speed of light in
can be achieved by a chiral route [1, 2]. In fact, chiral
vacuum. Assuming a time dependence of e-iωt, the RCP (+)
metamaterials also have other interesting properties, such as
wave and LCP (-) wave are defined as E ± = 1 E0 ( x ∓ i y ) 2
the giant optical activity and circular dichroism, which may
. The refractive indices for RCP and LCP waves can be
find their way into optical applications [3-8]. As an artificial metamaterial, CMM lacks any mirror symmetry so that the cross-coupling between the electric and magnetic fields exists at the resonance. The degeneracy of the two circularly polarized waves is thereby broken, i.e. right circularly polarized (RCP, +) waves and left circularly polarized (LCP, -) waves have different refractive indices. The chirality FIG. 1. (Color online) (a) Schematic of a unit cell of the
parameter κ describes the strength of the cross-coupling
chiral metamaterials consisting of four “U” split ring effect, so that the constitutive relations of a chiral medium is
resonators. (b) A photo of the experimental sample. The geometric parameters are given by ax=ay=15 mm, t=1.6 mm,
⎛ D ⎞ ⎛ ε 0ε −iκ / c ⎞ ⎛ E ⎞ ⎜ ⎟ = ⎜ iκ / c μ μ ⎟ ⎜ ⎟ , ⎝B⎠ ⎝ 0 ⎠⎝ H ⎠
d=1.5 mm, w=0.7 mm, and s=6 mm. The copper has a (1)
thickness of 0.03 mm.
n ± = n ± κ , where n = εμ
. When κ is
In order to study the transmission behaviors of the chiral structure, in our simulation and experimental works, a
n+ or n− becomes negative. At the
linearly polarized electromagnetic wave (E field in the x
same time, both RCP and LCP waves have the same
direction) is incident on the chiral structure. On the other side
μ / ε , where z0 is the impedance of
of the structure, we measured the transmitted field in the x
large enough, either
impedance of z / z0 =
and y polarizations (Txx and Tyx). Due to the four-fold
rotational symmetry, circular polarization conversion is
Since the beginning of the proposal of metamaterials,
absent. The transmission of circularly polarized waves can be
split ring resonators (SRRs) have played an important role in
converted from the linear transmission coefficients Txx and
achieving negative permeability. Experiments showed that
T ± = Txx ± iTyx . For the transmitted EM wave,
SRRs can be used as magnetic metamaterials even at infrared
and visible frequencies [11-13]. Furthermore, a magnetic
the polarization azimuth rotation angle θ can be calculated as
dimer can be formed by stacking two mutually twisted SRRs,
θ = [arg(T + ) − arg(T − )] / 2 . The ellipticity of the transmitted
and an array of these magnetic dimers can possess optical
wave is defined as η = arctan[( T + − T − ) /( T + + T − )] ,
activity [14, 15]. However, due to the lack of the rotational
which also measures circular dichroism.
symmetry, the optical activity is sensitive to the linear polarization of the incident wave. To eliminate this shortage, we propose here a design in which the U-shaped SRR pairs are arranged in C4 symmetry (see Fig. 1). Thus, the constructed CMM is effectively uniaxial for the normal incidence wave. A related retrieval procedure [6,16,17] can then be applied to calculate the effective parameters for our CMMs. Figure 1 shows the schematics of the CMMs we study. The unit cell of the CMM structure consists of doublelayered four “U” split ring resonators (Four-U-SRRs) patterned on opposite sides of an FR-4 board. This structure has been mentioned theoretically  and is discussed in another papers [19, 20]. The relative dielectric constant of the FR-4 board is 4.0 with a dielectric loss tangent of 0.025. The two layers of Four-U-SRRs are mutually twisted by 90 degrees. The Four-U-SRRs are arranged so that the CMM
FIG. 2. (Color online) Simulation and experimental results
structure possesses C4 symmetry. The dimensions of the unit
for the chiral metamaterial. (a) and (b) are the transmission
cell and the photo of our experimental sample are shown in
spectra for RCP and LCP waves. (c) and (d) are the
Fig.1 and the caption.
polarization azimuth rotation angle θ. (e) and (f) are the
In order to study the behavior of the chiral structure, we
ellipticity angle η of the transmitted wave.
conducted numerical simulations and experiments. The simulation works were carried out by using CST microwave
Figure 2(a) and 2(b) show the simulated and measured
studio (Computer Simulation Technology GmbH, Darmstadt,
transmission spectra. There are obvious differences between
Germany), wherein the finite integration technique was
the transmissions of RCP and LCP waves around the
applied. The periodic boundary conditions were applied to
resonances. Around the frequency of 5.1 GHz, the
the x and y directions, and the absorbing boundary conditions
transmission of LCP wave is 7~8 dB higher than that of the
were applied to the z direction. In the experiment, we
RCP wave. While around the frequency of 6.3 GHz, the
fabricated the chiral structures with a dimension of 20 by 20
transmission of the LCP wave is around 3~4 dB lower than
unit cells. The transmission coefficient was measured by an
that of the RCP wave. The fluctuations on the experiment
HP-8510C network analyzer with two standard horn antennas.
curve come from the multiple reflections between the CMM structure and the horn antennas.
Figures 2(c) to 2(f) show the simulated and experimental
and Figs. 3(c-d), due to the relation of
results of the polarization azimuth rotation angle θ and the
n± = n ± κ
strong chirality κ can push the refractive index of RCP (LCP)
ellipticity η of the transmitted wave. It can be clearly seen
wave to be negative around the resonant frequency of 5.1
that, in the middle of the two resonant frequencies, the
(6.4) GHz as shown in Fig. 3(c-d). However, due to the
ellipticity η = 0, where corresponds a pure optical activity
losses in the dielectric board, the figure of merit [–
effect, i.e. for the linear polarization incident wave, the
Re(n)/Im(n)] is only around 1.1 (1.3) at 5.1 (6.4) GHz in the
transmission wave is still the linear polarization but with a
negative index band. By using a lower loss substrate, the
rotated angle θ. The azimuth rotation angle θ is as large as
imaginary part of the negative index can be reduced. The
26o at 5.5 GHz. The rotation angle θ per wavelength is 700o/λ.
figure of merit can be larger than 10 (not shown here). In Figs. 3(e-f), we show the retrieved real parts for the permittivity and permeability of the CMM. Obviously, the Re(μ) is always positive throughout the entire frequency range (except the tiny range around 6.4GHz), while Re(ε) is negative in the frequency ranges above the two resonances. In traditional metamaterials, this will not result in a negative index. Therefore, the negative index of RCP (LCP) wave is actually attributed to the relatively small n and large chirality
FIG. 3. (Color online) The retrieved effective parameters of the chiral metamaterials based on the simulation (left) and experimental (right) data. (a-b) show the real parts of the
FIG. 4. (Color online) The current distributions driven by
refractive index n and chirality κ. (c-d) shows the real parts
the electric field in the x direction at 5.1 GHz and 6.3
of the refractive indices for RCP and LCP waves. (e-f)
GHz. The arrows in the middle of the SRRs show the
shows the real parts of the permittivity ε and permeability
direction of the x component of the induced magnetic
Figure 3 shows the retrieved effective parameters based
In order to understand the mechanism of the resonances
on the simulation and experimental data of the transmission
for our Four-U-SRRs CMM, we study the current modes on
and reflection for one layer of the CMMs. In the retrieval
the Four-U-SRRs. Fig. 4 shows the simulated current modes
process, the effective thickness of the CMM is assumed to be
at 5.1 GHz and 6.3 GHz driven by the electric field in the x
1.8 mm along the wave propagation direction. The chirality
direction. At 5.1 GHz, the currents on the top and bottom
is very large, e.g. it’s 2.15 at η = 0. If using the following
Four-U-SRRs are in the same direction. On the contrary, at 6.3 GHz, the currents on the top and bottom are in the
Ωκ 1ωκ 1ω Ωκ 2ωκ 2ω + ω − ωκ21 + iΓκ 1ωκ 1ω ω 2 − ωκ2 2 + iΓκ 2ωκ 2ω
opposite direction. According to the current distribution, we
can analyze the induced magnetic field. Fig. 4 shows that the
x component of the induced magnetic field Hx is nonzero.
to fit the result of the chirality κ , it gives us Ωκ 1 = 0.22,
ωκ 1 = 5.08
Γκ 1 = 0.02,
ωκ 2 = 6.42 GHz, Γκ 2 = 0.03 .
And moreover, at 5.1 GHz, Hx and Ex are in the opposite
Ωκ 2 = 0.28,
directions, while at 6.3 GHz, they are in the same direction.
Comparing Figs. 3(a-b)
11. C. Enkrich, M. Wegener, S. Linden, S. Burger, L.
This causality between electric and magnetic fields is
Zschiedrich, F. Schmidt, J. F. Zhou, Th. Koschny, and
consistent with the constitute equation Eq. (1).
C. M. Soukoulis, Phys. Rev. Lett. 95, 203901 (2005).
In summary, by twisting the four “U” split ring resonators in the propagation direction, which owns the fourfold
12. S. Linden, C. Enkrich, M. Wegener, J. Zhou, T.
rotational symmetry, a uniaxial chiral metamaterial can be
Koschny, and C. M. Soukoulis, Science 306, 1351 (2004).
constructed. We study the structure via the numerical simulation and the experiment at 3.5~7.5 GHz.
13. I. Sersic, M. Frimmer, E. Verhagen, and A. F.
simulation results agree with the experimental results very
Koenderink, Phys. Rev. Lett. 103, 213902 (2009).
well. This artificial structure gives us so strong chirality that
14. H. Liu, D. A. Genov, D. M. Wu, Y. M. Liu, Z. W. Liu,
the refractive index of RCP or LCP can be pushed to be
C. Sun, S. N. Zhu, and X. Zhang, Phys. Rev. B. 76,
negative at the vicinity of the resonance. Such structure can be scaled to other frequencies.
The proposed chiral
15. N. Liu, H. Liu, S. Zhu, and H. Giessen, Nat. Photonics
structures are suitable for planar fabrication. In the future, we
3, 157 (2009).
can use this planar design to contracture bulk chiral
16. D. H. Kwon, D. H. Werner, A. V. Kildishev, and V. M.
metamaterials via layer-by-layer method.
Shalaev, Opt. Express 16, 11822 (2008).
This work is supported by the European Union under
17. C. Menzel, C. Rockstuhl, T. Paul, and F. Lederer, Appl.
the projects EU-PHOME and EU-ECONAM, and TUBITAK
Phys. Lett. 93, 233106 (2008).
under the Project Nos., 107A004, and 107A012. One of the
18. N. Liu and H. Giessen, Opt. Express 16, 21233 (2008).
authors (E.O.) also acknowledges partial support from the
19. X. Xiong, W. H. Sun, Y. J. Bao, M. Wang, R. W. Peng,
Turkish Academy of Sciences. Rongkuo Zhao acknowledges
C. Sun, X. Lu, J. Shao, Z. F. Li, and N. B. Ming, Phys.
the China Scholarship Council (CSC) for financial support.
Rev. B 81, 075119 (2010). 20. R. Zhao, Th. Koschny, E. N. Economou, C. M.
J. B. Pendry, Science 306, 1353 (2004).
S. Tretyakov, I. Nefedov, A. Sihvola, S. Maslovski, and
Soukoulis, Phys. Rev. B 81, 235126 (2010).
C. Simovski, J. Electromagn. Waves Appl. 17, 695 (2003). 3.
A. V. Rogacheva, V. A. Fedotov, A. S. Schwanecke, and N. I. Zheludev, Phys. Rev. Lett. 97, 177401 (2006).
B. Wang, J. Zhou, T. Koschny, and C. M. Soukoulis, Appl. Phys. Lett. 94, 151112 (2009).
S. Zhang, Y.-S. Park, J. Li, X. Lu, W. Zhang, and X. Zhang, Phys. Rev. Lett. 102, 023901 (2009).
E. Plum, J. Zhou, J. Dong, V. A. Fedotov, T. Koschny, C. M. Soukoulis, and N. I. Zheludev, Phys. Rev. B 79, 035407 (2009).
J. Zhou, J. Dong, B. Wang, T. Koschny, M. Kafesaki, and C. M. Soukoulis, Phys. Rev. B 79, 121104(R) (2009).
M. Decker, M. Ruther, C. E. Kriegler, J. Zhou, C. M. Soukoulis, S. Linden, and M. Wegener, Opt. Lett. 34, 2501 (2009).
J. D. Jackson, Classical Electrodynamics, 3rd ed. (Wiley, New York, 1998).
10. J. A. Kong, Electromagnetic Wave Theory (EMW Publishing, Cambridge, MA, 2008).